Presentation on theme: "Calculation of optical properties and macroscopic polarization with SIESTA Daniel Sánchez-Portal Centro de Física de Materiales, Centro Mixto CSIC- UPV/EHU,San."— Presentation transcript:
Calculation of optical properties and macroscopic polarization with SIESTA Daniel Sánchez-Portal Centro de Física de Materiales, Centro Mixto CSIC- UPV/EHU,San Sebastián, Spain Efficient density-functional calculations with atomic orbtitals: a hands-on tutorial on the SIESTA code CECAM Tutorial Lyon, June 18-22
Polarizability Exact many body wavefunctions and eigenvalues Approximation with Kohn-Sham orbitals and eigenvalues Molecule
Dielectric function in solids Without local field corrections Unfortunately there is no way to apply this formula to a solid Position operator is ill-defined for extended wavefunctions
A word of caution for non-local potentials No problem: localized objects
Thomas-Reiche-Kuhn or f-sum rule Drude term for metals (ω 0)
Parameters and input OpticalCalculation : default.false., set to.true. Optical.NumberOfBands : all of them used if not specified %block Optical.Mesh n 1 n 2 n 3 %endblock Optical.Mesh Optical.Broaden: small “artificial” broadening, 0.X eV Optical.PolarizationType: polarized, unpolarized, polycrystal %block Optical.Vector E x E y E z %endblock Optical.Vector Either E, electric field or k, propagation vector
Optical.Vector Polarized: Unpolarized: Polycrystal: Average over three spatial directions
What is left out in this approach *Classical collective modes (plasmons). They can be included at the RPA level. Important at low energies for small systems, not that much for bulk. *Excitonic effects (electron-hole interaccion). Quite hard to include *Spectrum beyon Kohn-Sham approx. At the moment just the “scissor operator” to correct excitation energies.
Diamond and Silicon Silicon Diamond SIESTA G.F. Bertsch et al.Phys.Rev. B 62, 7998 (2000). PW, CASTEP DZP basis set (26 bands)
Optical response of 4-Å diameter SWCNT with SIESTA Testing the accuaracy of SIESTA band structures on graphene: Including a diffuse 3s orbital we have perfect with PW up to 6 eV Adding an additional 3p shell the agreement is extended to eV Our band structures for the 4-Å are in very nice agreement with the PW calculations of Li et al. In fact,...
Optical response of 4-Å diameter SWCNT with SIESTA (cont.) (3,3) (4,2) (5,0) (4,2) (3,3) All channels occupied f=2x :0.7:0.2 (5,0):(3,3):(4,2)